Available online at www.sciencedirect.com
Journal of Power Sources 174 (2007) 1041–1045
Composite anode materials for Li-ion batteries Zhaoyin Wen ∗ , Xuelin Yang, Shahua Huang Shanghai Institute of Ceramics, Chinese Academy of Sciences, 1295 Ding Xi Road, Shanghai 200050, PR China Available online 23 June 2007
Abstract The Si (Li4 Ti5 O12 )/Ag composites were synthesized by electroless deposition (ED), and amorphous carbon was incorporated into Si and Li4 Ti5 O12 by dehydration reaction using concentrated H2 SO4 as dehydration agent and thermal decomposition of sucrose for the preparation of Si(Li4 Ti5 O12 )/C composites. The Si/Ag(C) composite electrodes demonstrated superior cyclabilities owing to the improvement of electronic conductivity; meanwhile, the high-rate capability of Li4 Ti5 O12 electrode was also greatly improved after incorporation of silver and amorphous carbon. © 2007 Elsevier B.V. All rights reserved. Keywords: Lithium-ion battery; High-rate performance; Li4 Ti5 O12 /Ag; Li4 Ti5 O12 /C; Si/Ag; Si/C
1. Introduction Recently, various anode materials with improved reversible capacity and stability over commercial graphite have been highly proposed for Li-ion batteries. Silicon is an attractive one because of its largest capacity; spinel Li4 Ti5 O12 is another candidate owing to its superior structural stability [1,2]. However, the application of silicon is hindered by its poor conductivity and drastic volume changes , and low-rate capability resulted from low electronic conductivity also limited the practical use of Li4 Ti5 O12 . Conductive fillers are routinely added to electrodes to compensate for the low electronic conductivity of electrode active materials and achieve good results. With the presence of conductive additives, the power and cycle life of the battery could be significantly augmented [5,6]. It was found in our previous study that Li4 Ti5 O12 /Ag [7,8] prepared by solid-state reaction was very useful to improve the high-rate performance of Li4 Ti5 O12 . In this study, silver with particle size less than 100 nm was further incorporated into Li4 Ti5 O12 and Si by a chemical deposition to study its influence on cycling ability of Li4 Ti5 O12 and Si. Furthermore, amorphous carbon, as another conductive additive was also incorporated into Li4 Ti5 O12 and Si using solid-state reaction and liquid-phase reaction, respectively. Compared with bare silicon and Li4 Ti5 O12 , Si/Ag (Si/C) composites could exhibit
Corresponding author. E-mail address: [email protected]
0378-7753/$ – see front matter © 2007 Elsevier B.V. All rights reserved. doi:10.1016/j.jpowsour.2007.06.041
better cyclability and Li4 Ti5 O12 /Ag (Li4 Ti5 O12 /C) also showed greatly improved high-rate capability. 2. Experiments 2.1. Synthesis of Si (Li4 Ti5 O12 )/Ag composite The (90 wt% Si)/(10 wt% Ag) and (93.7 wt% Li4 Ti5 O12 )/ (6.3 wt% Ag) composites were synthesized by ED. Dilute NH3 • H2 O was titrated in 1 M aqueous solution of AgNO3 until the deposit disappeared, and a colorless solution was therefore obtained. The above solution obtained and dilute CH3 CHO was dropped simultaneously into the suspension of Li4 Ti5 O12 prepared by solid-state reaction method at 850 ◦ C for 12 h or commercial silicon powders with vigorous magnetic stirring at 80 ◦ C. To suppress the sustained growth of silver particles, magnetic stirring was performed throughout the reduction process. The deposited powders were washed with distilled water and dried under vacuum at 100 ◦ C for 12 h [9,10]. 2.2. Synthesis of Si(Li4 Ti5 O12 )/C composite (20 wt% Si)/(80 wt% C) and (95 wt% Li4 Ti5 O12 )/(5 wt% C) composites were prepared by dehydration reaction using concentrated H2 SO4 as dehydration agent and thermal decomposition of sucrose, respectively. Commercial silicon powders were homogeneously dispersed in a sucrose solution with the help of an ultrasonic bath, and the obtained suspension was further agitated under infrared light until it was converted into
Z. Wen et al. / Journal of Power Sources 174 (2007) 1041–1045
syrup. The concentrated H2 SO4 was slowly added into the asprepared syrup, mixed homogeneously and dehydrated for 2 h. The resulting product was filtered after dilution by distilled water. Then it was rinsed with distilled water until pH 7 was reached and dried under vacuum for 8 h, ground and sieved . The as-mentioned pristine Li4 Ti5 O12 powders were homogeneously dispersed in the aqueous solution of sucrose with the help of an ultra sonic bath and the obtained suspension was then further agitated with gentle heating until it converted into syrup. Then, the samples were heated in a muffle furnace at 950 ◦ C for 2 h in N2 and cooled down to room temperature naturally. The powders obtained were finally ground. 2.3. Measurements X-ray diffraction (XRD) was used to analyze the phases formed. Electron back-scatter diffraction (EBSD) mapping analysis system and transmission electron microscopy (TEM) were, respectively, used to observe silver and silicon distribution. The composite electrodes for electrochemical test were made of the Si-based composite (85 wt%), acetylene black (10 wt%) and polyvinylidene fluoride (PVDF) binder (5 wt%) homogeneously mixed in N-methyl pyrrolidinone (NMP) solvent by ball milling and then coated uniformly on a copper foil. For the Li4 Ti5 O12 -based composite, the electrode ingredient was 85%:7%:8% in weight ratio and coated on an aluminum foil. Finally, the electrode was dried under vacuum at 100 ◦ C for 10 h. The charge and discharge capacities were measured with a coin cell (2025 type), in which a lithium metal foil was used as the counter electrode. The electrolyte employed was 1 M LiPF6 in ethylene carbonate and dimethyl carbonate solution (EC + DMC) (1:1). Cell assembly was carried out in an argonfilled glove box (VAC AM-2). The Si-based composite electrode was cycled in the voltage range from 0.02 to 1.5 V employing a constant current density of 0.1 mA cm−2 , and Li4 Ti5 O12 -based composite electrode was cycled between 0.5 and 2.3 V at the rate of 2C. 3. Results and discussion The XRD patterns (Fig. 1) of Si/Ag and Li4 Ti5 O12 /Ag composites showed that except the characteristic patterns of elemental silver, all diffraction peaks were in accordance with the patterns of silicon and spinel Li4 Ti5 O12 , and all patterns in Si/C and Li4 Ti5 O12 /C composite samples were attributed to silicon and Li4 Ti5 O12 indicating an amorphous feature of incorporated carbon. The TEM image of Si/Ag and the EBSD image of the Li4 Ti5 O12 /Ag composite obtained by ED method are shown in Fig. 2a and b, respectively. It was clearly observed that nano-sized silver particles with size less than 100 nm were uniformly distributed on the surface of silicon and Li4 Ti5 O12 particles. Compared with the solid-state reaction [7,8] and the direct reduction of AgNO3 in other papers , the complex reduction, obviously, could produce much smaller conductive particles with narrow size distribution. It was therefore assumed that these highly dispersed nano-sized silver particles could
Fig. 1. XRD patterns of (a) the Si (Li4 Ti5 O12 )/Ag composites and (b) the Si (Li4 Ti5 O12 )/C composites.
play a positive role in improve electrical contact between silicon (Li4 Ti5 O12 ) particles and current collector. Accordingly, the discharge/charge performance of Si/Ag and Li4 Ti5 O12 /Ag composite electrode would benefit from the good conducting network between active particles. Fig. 3a shows the TEM image of Si/C prepared by lowtemperature carbonization. The silicon particle size was less than 25 nm, with a distinct contrast from the carbon matrix as seen from the image. Therefore, we can conclude that the amorphous carbon with good electronic conductivity formed a conduction pathway for electrochemical reactions. On the other hand, nano-sized silicon particles with small absolute volume changes were embedded in carbon matrix, therefore, there was no direct contact between silicon particles, and the electrochemical sintering process transformed from silicon nanoparticles into dense blocks was suppressed to the utmost of degree. Fig. 3b shows the EBSD image of the Li4 Ti5 O12 /C obtained by thermal decomposition of sucrose. Two kinds of particle morphologies existed in the composite, one ascribed to Li4 Ti5 O12 phase, another one, nano-sized and flaky featured, therefore attributed to carbon phase. The average thickness of the flakes was below 50 nm. It was suggested that the nano-sized carbon flakes resided in the void of active powders and formed a conduction pathway which was essential to improve the utilization of the active material Li4 Ti5 O12 . Fig. 4a compares the first discharge/charge voltage curves of pure silicon, Si/Ag composite and Si/C composite elec-
Z. Wen et al. / Journal of Power Sources 174 (2007) 1041–1045
Fig. 2. (a) TEM images of the Si/Ag composite and (b) SEM images of the Li4 Ti5 O12 /Ag composite.
Fig. 3. (a) TEM images of the Si/C composite and (b) SEM images of the Li4 Ti5 O12 /C composite.
trodes cycled at a constant current density of 0.1 mA cm−2 . The pure silicon electrode delivered a large specific capacity of 3973 mAh g−1 , which was much close to its theoretical value, but only 73% of it could be reversibly extracted. After the addition of silver, the first discharge capacity dropped to 2729 mAh g−1 with an improved columbic efficiency of 86%, that is to say, extraction depth of Li+ from silicon could be furthered with the help of silver. The release of polarization between discharge and charge process benefited from the Agimproved conducting network. In the case of Si/C composite, 80 wt% of carbon was added into silicon powders, but the composite electrode still demonstrated a large discharge capacity of 1209 mAh g−1 because of relative light mass of carbon compared with silver. The decreased columbic efficiency may be related to the absorbed –OH group which would irreversibly trap Li+ in the first cycle. The initial capacity drop was an excepted
phenomenon in common disordered carbon, but it could be avoided with increase of cycling. As shown in Fig. 4b, the first discharge capacity of pristine Li4 Ti5 O12 , Li4 Ti5 O12 /Ag composite and Li4 Ti5 O12 /C composite electrodes cycled at the rate of 2C was 162.2, 244.2 and 219.1 mAh g−1 . There were two platforms for every sample, the main discharge platform of pristine Li4 Ti5 O12 and the Li4 Ti5 O12 /C composite at the first cycle was 1.53 V, but the Li4 Ti5 O12 /Ag composite was 1.45 V. The Ag and C additives greatly improved the first discharge capacity. Metal silver mainly increased the capacity at about 1.5 V platform, while amorphous carbon increased the capacity at both 1.5 and 0.5 V platforms. Fig. 5a shows the charge capacity and columbic efficiency versus cycle number for pure silicon, Si/Ag composite and Si/C composite electrodes cycled at a constant current density (0.1 mA cm−2 ). As shown in Fig. 5a, the pure silicon electrode
Z. Wen et al. / Journal of Power Sources 174 (2007) 1041–1045
Fig. 5. Variation of the charge capacities for (a) the pure Si and the Si/Ag(C) composite and discharge capacities for (b) the pristine Li4 Ti5 O12 and the Li4 Ti5 O12 /Ag(C) composite. Fig. 4. (a) The first charge–discharge curves of the pure Si and the Si/Ag(C) composite. (b) The first discharge curves of the pristine Li4 Ti5 O12 and the Li4 Ti5 O12 /Ag(C) composite.
faded almost all of its first capacity within only five cycles. After the addition of silver and carbon additives, the Si/Ag composite electrode remained a capacity above 500 mAh g−1 and the Si/C composite electrode delivered a stable reversible capacity near to 1000 mAh g−1 without obvious capacity fading after 30 cycles, which was expected as a result of the increase of electronic contact, meanwhile, possible volume changes of silicon particles during repeated cycling were also effectively absorbed by amorphous carbon matrix. These results were in good consistency with other reports [11,13,14]. The cycling behaviors of the pristine Li4 Ti5 O12 , Li4 Ti5 O12 /Ag composite and Li4 Ti5 O12 /C composite are shown in Fig. 5b. The 50th discharge capacities were 153, 196.2 and 178.9 mAh g−1 with the capacity degradations of 2.67, 3.59 and 3.19% compared to the second cycle for the pristine Li4 Ti5 O12 , Li4 Ti5 O12 /Ag composite and Li4 Ti5 O12 /C composite, respectively. The Ag and C additive greatly improved the reversible capacity of the pristine Li4 Ti5 O12 , although the capacity degradation of the Li4 Ti5 O12 /Ag(C) composite was bigger than the pristine Li4 Ti5 O12 at the rate of 2C, its absolute value of discharge capacity after 50 cycles was much higher than the precursor. The greatly increased reversible capacity of Li4 Ti5 O12 /Ag(C) composite could be attributed to the improvement of cathode
utilization. The Ag and C additive resided in the surface of the Li4 Ti5 O12 matrix and formed a conduction pathway which was essential to improve the electronic conductivity of the electrode and the utilization of the Li4 Ti5 O12 material, leading to improvement in charge and discharge performance and furthermore the cycle life of the battery. 4. Conclusions The Ag and C additives were useful to improve the electrochemical performance of silicon and Li4 Ti5 O12 . The Si/Ag and Si/C composite electrodes demonstrated superior cyclabilities owing to the improvement of electronic conductivity and effective buffering of volume changes, meanwhile, the high-rate capability of Li4 Ti5 O12 electrode was greatly improved after incorporation of silver and carbon. Acknowledgments This work was financially supported by National Science Foundation of China (projects No. 20333040 and 50672114) and 863 project of China No. 2006AA03Z232. References  W.J. Weydanz, M.W. Mehrens, R.A. Huggins, J. Power Sources 81–82 (1999) 237–242.
Z. Wen et al. / Journal of Power Sources 174 (2007) 1041–1045  D. Peramunge, K.M. Abhamm, J. Electrochem. Soc. 145 (1998) 2609–2615.  Z.P. Guo, J.Z. Wang, H.K. Liu, S.X. Dou, J. Power Sources 146 (2005) 448–451.  C.H. Chen, J.T. Vaughey, A.N. Jansen, D.W. Dees, et al., J. Electrochem. Soc. 148 (2001) A102–A104.  D. Guyomard, J.M. Tarascon, Solid State Ionics 69 (3–4) (1994) 222–237.  Z.X. Shu, R.S. McMillan, J.J. Murray, J. Electrochem. Soc. 140 (4) (1993) 922–927.  S.H. Huang, Z.Y. Wen, X.J. Zhu, Z.H. Gu, Electrochem. Commun. 6 (2004) 1093–1097.  S.H. Huang, Z.Y. Wen, J.C. Zhang, Z.H. Gu, X.H. Xu, Solid State Ionics 177 (2006) 851–855.
 X.L. Yang, Z.Y. Wen, S.H. Huang, X.J. Zhu, X.F. Zhang, Solid State Ionics 177 (2006) 2611–2615.  S.H. Huang, Z.Y. Wen, X.L. Yang, X.J. Zhu, B. Lin, Electrochem. SolidState Lett. 9 (2006) A443–A447.  X.L. Yang, Z.Y. Wen, X.J. Zhu, S.H. Huang, Electrochem. Solid-State Lett. 8 (2005) A481–A483.  X.D. Wu, Z.X. Wang, L.Q. Chen, X.J. Huang, Electrochem. Commun. 5 (2003) 935–939.  J.W. Kim, J.H. Ryu, K.T. Lee, S.M. Oh, J. Power Sources 147 (2005) 227–233.  J.H. Ryu, J.W. Kim, Y.E. Sung, S.M. Oh, Solid-State Lett. 7 (2004) A306–A309.